Abstract
The structural and mechanical stability of Fe_{2}TaAl and Fe_{2}TaGa alloys along with the electronic properties are explored with the help of density functional theory. On applying different approximations, the enhancement of semiconducting gap follows the trend as GGA < mBJ < GGA + U. The maximum forbidden gaps observed by GGA + U method are E_{g} = 1.80 eV for Fe_{2}TaAl and 1.30 eV for Fe_{2}TaGa. The elastic parameters are simulated to determine the strength and ductile nature of these materials. The phonon calculations determine the dynamical stability of all these materials because of the absence of any negative frequencies. Basic understandings of structural, elastic, mechanical and phonon properties of these alloys are studied first time in this report.
Similar content being viewed by others
Introduction
Significant momentum in the study of intermetallic Heusler alloys has increased over the last decade as these systems exhibit numerous extraordinary capabilities in exposing the desired properties, extending from robust spinpolarization, halfmetallic magnetism, magnetoresistance, shape memory effect, spin gapless semiconductor to giant magnetocaloric effect, phase transitions and thermoelectric effect^{1,2,3,4,5,6,7}. The technological applications exploiting these properties have been achieved successfully. Spintronic and thermoelectric applications are the offshoots of halfmetallic ferromagnetism (being castoff in spin injectors^{8}, spin filters^{9}, magnetic tunnel junctions^{10}, spin valves^{11}, random access memories^{12}) and spin gapless attributes to the Seebeck effect useful for thermoelectric devices^{13}. Within these dimensions, the materials with compatible lattice structure, high spin polarization and high Curie temperature are anticipated in practical spintronic applications. Magnetoelectronic devices mostly depend on the disproportionate number of majority and minority spin carriers, as exhibited ideally by halfmetallic materials i.e. 100% spin polarization at the Fermi level. Such materials display the concoction properties of semiconductor and metal. Additional motive to delegate Heusler alloys in these applications is that these systems have the same crystallographic structure with different functional characteristics and some of them are even very close in electronic structure and composition^{14,15}. Since the discovery of the NiMnSb Heusler alloy in 1983^{16}, a sequence of experimental as well as theoretical efforts (first principles simulations) were attempted to predict novel semiconductor or halfmetallic systems. Among such compounds, transition metal based Heuslers have been widely investigated by material scientists worldwide. Predominantly, the Fe based Heusler structures constitute a vast family with semiconducting or halfmetallic band profiles. For example, Fe_{2}YSi (Y=Cr, Mn, Fe, Co, Ni) alloys were experimentally synthesized and predicted to be halfmetallic alloys^{17}. Fe_{2}TiAl was reported to have thermoelectric applications^{18}. Other materials like, Fe_{2}TiSi, Fe_{2}TiGe and Fe_{2}ZrSi^{19}, FeMnSi^{20}, FeVRuSi^{21} and many more to report here have been investigated for their magnetic, semiconducting or mechanical properties. Using firstprinciple calculations, Fe_{2}YZ (Y=V, Ti, Nb, Zr, Ta, Hf and Z=Al, Ga, In, Sn, Ge, Si) Heusler compounds with room temperature power factors 4 to 5 times larger than classical thermoelectrics were reported recently by Bilc et al.^{22}. However, a little information is available on the electronic structure, mechanical stability, phonon dynamics and bonding characteristics of Fe_{2}TaAl and Fe_{2}TaGa alloys. In addition, the untouched lattice dynamical parameters and phonon properties are necessary to understand the intriguing physical properties and hence in this work, we tried to investigate their structural and mechanical stability, electronic and lattice dynamical properties in detail.
Results and Discussion
Structural and mechanical stability
FullHeusler ternary alloys of Fe_{2}TaAl and Fe_{2}TaGa type have been found to crystallize in a cubic structure with space group (Fm3m) as depicted in Fig. 1^{22}. The corresponding atomic locations are Fe (1/4, 1/4, 1/4), Ta (1/2, 1/2, 1/2) and Z (0, 0, 0). The ground state structure is determined by geometry optimization via the total energy per unit cell (see Supporting Information) and thereby the equilibrium lattice constants, derivative of bulk modulus, total energy and equilibrium volume are obtained as shown in Table 1. These optimized lattice parameters are fetched out to calculate the ground state properties of these alloys.
The mechanical stability and elastic response of any crystal system is measured from the elastic constants and thereby the indication of its mechanical properties; e.g Bulk/Young’s/shear moduli, Debye or melting temperature, poisons ratio, brittle/ductile or hardness, etc are derived from them. Macroscopic distortion of a crystal structure is directly related to the elastic constants and is applicable in the evaluation of elastic energies or strains in materials under applied (internal/external/thermal) stresses^{23}. These constants are determined by the linear response of a crystal towards the external forces, and are also associated with structural stability, equation of state (EOS), interatomic potential and phonon spectra^{24}. Beyond this, the thermal properties including specific heat, thermal expansion, Debye temperature and Gruneisen parameter are exclusively linked to elastic constants. Consequently, the determination of elastic constants is indispensable to characterize a solid crystal. In this work, we have calculated the elastic constants of Fe_{2}TaAl and Fe_{2}TaGa systems using the generalized gradient approximation (GGA) and are listed in Table 2. For a simple cubic system, the elastic stiffness constants (C_{ij}) are reduced to only three independent constants viz. C_{11}, C_{12}, and C_{44}. From Table 2, it can be seen that the comprehensive Born criteria; C_{12} < B < C_{11}, (C_{11} − C_{12}) > 0, (C_{11} + 2C_{12}) > 0 and C_{44} > 0 is rigorously followed by the observed lattice constants and hence their mechanical stability is confirmed^{25}. Further, to get the information about the different elastic moduli and other derivables, ViogtReussHill method is used via the Eqns (1–3)^{26,27,28},
where, bulk modulus is represented as,
and, the Youngs modulus, Poisson’s ratio and anisotropy parameter are defined as
Calculated results for the values of elastic parameters (B, G, Y, A, v, C”, B/G, etc.) are summed up in Table 2. The hardness of a material is generally delivered from the observed values of bulk modulus (B) and shear modulus (G). Indisputably, when a stress is applied to any system, the opposition offered at the critical point before which the system is fractured refers to the hardness of that material^{29}. Concurrently, the ductile and brittle character of materials is directly linked to the critical value (1.75) of B/G ratio. If B/G is less than the critical value, then the material is ductile otherwise it is said to be brittle^{30}. The covalent materials (e.g. Diamond) in principle are relatively hard and obviously brittle with a smaller Pugh ratio. The strong covalent bonds in such materials certainly produce a significant resistance resulting in a quite high hardness. Conversely, ductile materials with a high Pugh’s ratio are characterized by metallic bonding and low hardness. Consequently, the observed values of B, G and B/G clearly determine the Fe_{2}TaAl alloy to be much harder and ductile from Fe_{2}TaGa compound. This claim is also supported by the (C” = C_{12}–C_{44}) values because its positive value defines the ductile nature of the present alloys and if its value is negative, then the system is said to be brittle in nature^{31}. Positive Cauchy pressure also specify the presence of metallic bonding in a material while as the negative value demonstrates the directional (covalent) and angular bonds. In the present set of calculations, Cauchy pressure predicted for both the Heusler alloys are positive which reflects their metallic character. Poisson’s ratio and its critical value; 0 < υ < 0.5 simply defines the plasticity of a crystal. Its small value reflects the maximum plastic character and conversely, the material is elastic in nature^{32}. So, the elastic nature of these alloys can be observed from the υ values mentioned in Table 2. At the same time, the value of anisotropic factor (A) for a perfectly isotropic system is equal to 1 and its value below or above unity proposes the anisotropic character of a compound. Therefore, the Fe_{2}TaAl alloy is purely isotropic but the Fe_{2}TaGa alloy is anisotropic in nature^{31}.
The thermodynamic behavior of the Febased Heusler systems has been described by the calculation of melting temperature (T_{m}). Using the empirical equation (Eqn. 4) given below, the melting temperature of the present Heusler systems has been premeditated^{33,34}.
The large values of T_{m} as seen from the Table 2 imply the strength of the present materials against the temperature and this hints about the retention of their ground state crystal structures at raised temperatures.
Semiconducting gap and electronic structure
Since both these alloys have 24 valence electrons (Z_{t}) in their equilibrium structures, therefore, SlaterPauling rule^{34}; (M_{t} = Z_{t} − 24) comprises the zerospin magnetic moment for both these materials. Their nonmagnetic character has earlier been reported in ref.^{22}. The groundwork of structural optimization yields the equilibrium lattice constant, and the same is utilized to calculate the electronic band profile of Fe_{2}TaAl and Fe_{2}TaGa Heusler materials. Three different schemes; generalized gradient approximation (GGA), onsite Hubbard approximation (GGA + U) and modified Beckhe Johnson (mBJ) schemes have been employed and the spin polarized band profiles are displayed in Figs 2 and 3. The GGA and mBJ calculated energy gaps are very small as compared to GGA + U calculations. However, GGA + U clearly widens the gap between valence and conduction bands in both the compounds. From GGA + U calculations, Fe_{2}TaAl is observed to be a direct band gap material with Eg = 1.80 eV, while as Fe_{2}TaGa is observed to be indirect band gap semiconductor with the corresponding energy gap of 1.30 eV. In the latter case, the valence band maximum (VBM) occurs at the Γ symmetry point and the conduction band minimum (CBM) occurs at the X symmetry point in its Brillouin zone. However, GGA and mBJ methods reveal both these materials to be the ptype indirect band gap semiconductors.
Further, the spin polarized total density of states (TDOS) depicted in Fig. 4 and partial density of states (PDOS) shown in Fig. 5 for the present materials at their equilibrium lattice constants are discussed. Since, the total DOS in up and down spin channels are same (cancel each other), therefore the nonmagnetic character of these alloys can be estimated. Also, the pDOS of these materials by GGA underestimates the band structure and therefore small or negligible gaps are observed by this method. Consequently, the onsite Hubbard correction (described in section 4 for Fed states) widens the band gap comparatively. The Fed and Tad states are mostly populated around the Fermi level with a maximum contribution towards the total DOS and consequently, the corresponding bondingantibonding states control the energy gap formation. At the same time group IV atomic states are less active around the Fermi level in these materials. Thus, the observed band gap in these alloys is due to the typical dd hybridization between the valence states of Fe and Ta atoms and the same has been explained elsewhere for similar materials like Co_{2}TaAl and Co_{2}TaGa^{3,28}. Hence, from the observed band profiles and densities of state plots, both the compounds are found to be ptype indirect band gap semiconductors. Present calculations unlock the potential application of these alloys in semiconductor and energy harvesting technologies.
Phonon properties and Cohesive Energies
Phonon dispersions are interesting phenomenon to understand the dynamical stability of a crystal system above and beyond knowing their thermal behavior, superconductivity, Raman and thermal spectroscopy^{35,36,37}. Figure 6(a,b) shows the phonon dispersion curves (PDCs) of these alloys obtained using GGA scheme. The four atoms of Fe_{2}TaAl and Fe_{2}TaGa system in its unit cell give rise to three acoustical and nine optical modes constituting a total of 12 phonon branches. But, in different directions, this number is reduced due to degeneracy. The optical modes obtained for Fe_{2}TaAl are at around 510.19 cm^{−1} and 680.22 cm^{−1} and for Fe_{2}TaGa are around 470.29 cm^{−1}, 590.63 cm^{−1} at zone center Г and W points.
It can also be seen from Fig. 4(a,b) that the longitudinal opticaltransverse optical (LOTO) splitting in our materials is almost nil at Г and W symmetry points. The difference of LO and TO (ω_{LO} − ω_{TO}) is called a reststrahlen band, which estimates the number of reflected electromagnetic waves. In our calculation \({\omega }_{LO}^{2}{\omega }_{TO}^{2}\approx 0\) at Г and W points, hence exhibit higher phonon scattering ability. Such phenomenon can obviously enhance the thermoelectric response of these materials by decreasing thermal conductivity. The dynamical stability is confirmed by the absence of imaginary frequency in all high symmetry direction for both the investigated compounds.
Since, the stability of both these materials has been confirmed via Convex Hull analysis with −303.3 MeV for Fe_{2}TaAl and −64.3 MeV for Fe_{2}TaGa as the energy above the hull which is equal to the energy of formation of the compounds of interest from the phases that would be stable if the compound did not exist^{22}. Therefore, our phonon results strengthen the stability criteria of these alloys. Moreover, we have calculated the cohesive energies (E_{coh}) of these compounds using the following equation:
where \({E}_{Fe}^{iso}\), \({E}_{Ta}^{iso}\) and \({E}_{Al/Ga}^{iso}\) are the isolated atomic energies of the Fe, Ta and Al/Ga atoms, respectively, and \({E}_{F{e}_{2}TaAl/Ga}^{Total}\), is the total energy of Fe_{2}TaAl and Fe_{2}TaGa per formula unit. The measurement of strength of the binding force between the constituent atoms in a solid structure is confirmed from cohesive energy its positive value indicates the stability of the material. The calculated values of the cohesive energy are 22.71 eV for Fe_{2}TaAl compound and 20.67 eV for Fe_{2}TaGa alloy. These observed values are significant and comparable to Co_{2}TaSi (21.76 eV), Co_{2}TaGe (19.18 eV)^{38} and Hf_{2}Val (21.56 eV)^{39}; and this specifies the large value of chemical bond energy. Therefore, the stability of the present materials is confirmed from the mechanical stability criteria, cohesive energy and phonon dispersion results.
Conclusion
In this study, the electronic and mechanical properties of cubic Fe_{2}TaAl and Fe_{2}TaGa alloys have been examined using the density functional theory. Calculations of the electronic structure shows the indirect band gaps along ΓL symmetry for all these materials. These compounds directly fall under the Slater Pauling rule that depicts their semiconducting behavior. Thus, we have confirmed from our studies that these fullHeusler alloys are narrow band gap semiconductors with 0.80 eV for Fe_{2}TaAl and 0.61 eV for Fe_{2}TaGa. In relation to electronic structure, the mechanical properties have been calculated. A theoretical study predicts the hardness and ductile nature of these materials and their ductility increases from Al > Ga and are potentially the possible hard semiconductor materials. In this study, the electronic, phonon and mechanical properties of cubic Fe_{2}TaAl and Fe_{2}TaGa alloys have been examined using the density functional theory. The calculation of lattice vibrations from DFPT gives the phonon dispersion. The coupling of optical and acoustic mode is an interesting phenomenon that we have observed in this study with zero LOTO splitting at Г and W points of symmetry. The zero value of reststrahlen band is responsible for higher value of phonon scattering and reduced the lattice thermal conductivity.
Methodology
The investigation of structural, elastic, electronic and phonon properties of the Fe_{2}TaAl and Fe_{2}TaGa compounds, firstprinciples calculations using the full potential linearized augmented planewave method (FPLAPW)^{40} as executed in the WIEN2k Package^{41}. This quantum mechanical code can precisely simulate the ground state structure, band gaps, dielectric properties, magnetic properties, and so on. The generalized gradient approximation (GGA)^{42}, mBJ^{43} and onsite Hubbard correction (GGA + U)^{44}, were adopted for the exchangecorrelation potentials. In GGA + U calculations, we have used the UJ = 4.0 eV for Fed electrons with J = 0 according to the Dudarav’s method^{45}. A dense kpoint mesh of 10 × 10 × 10 was used in the Brillouin zone integrations. The basis functions are expanded up to R_{MT}K_{max} = 7, where RMT is the smallest atomic radius in the unit cell and K_{max} refers to the magnitude of the largest k vector in the plane wave expansion. The total energy convergence tolerance for the calculations was selected within 1 × 10^{−6} eV. Furthermore, the elastic properties were calculated by cubic elastic code^{46} and from these elastic constants other mechanical parameters were determined to discuss the mechanical response of these materials. DFT has proven to be one of the successful methods to predict the stability as well as ground state properties of the materials theoretically^{47,48}. The lattice dynamical properties were analyzed in term of phonon frequencies as a secondorder derivative of the total energy with respect to atomic displacements within the frame work of DFPT^{49} by using the Quantum Espresso package^{50}.
References
Galanakis, I., Dederichs, P. H. & Papanikolaou, N. SlaterPauling behavior and origin of the halfmetallicity of the fullHeusler alloys. Phys. Rev. B 66, 174429 (2002).
Özdoğan, K., Şaşıoğlu, E. & Galanakis, I. SlaterPauling behavior in LiMgPdSntype multifunctional quaternary Heusler materials: Halfmetallicity, spingapless and magnetic semiconductors. J. Appl. Phys. 113, 193903 (2013).
Khandy, S. A. & Gupta, D. C. DFT investigations on mechanical stability, electronic structure and magnetism in Co_{2}TaZ (Z=Al, Ga, In) heusler alloys. Semicond. Sci. Technol. 32, 125019 (2017).
Planes, A., Mañosa, L. & Acet, M. Magnetocaloric effect and its relation to shapememory properties in ferromagnetic Heusler alloys. J. Phys.: Condens. Matter 21, 233201 (2009).
Do, D., Lee, M. S. & Mahanti, S. D. Effect of onsite Coulomb repulsion on thermoelectric properties of fullHeusler compounds with pseudogaps. Phys. Rev. B 84, 125104 (2011).
Winterlik, J., Fecher, G. H., Thomas, A. & Felser, C. Superconductivity in palladiumbased Heusler compounds. Phys. Rev. B 79, 064508 (2009).
Lin, T. T. et al. Antisiteinduced diverse diluted magnetism in LiMgPdSbtype CoMnTiSi alloy. Sci. Rep. 7, 42034 (2017).
Saito, T., Tezuka, N., Matsuura, M. & Sugimoto, S. Spin injection, transport, and detection at room temperature in a lateral spin transport device with Co_{2}FeAl_{0.5}Si_{0.5}/nGaAs schottky tunnel junctions. Appl. Phys. Exp 6, 103006 (2013).
Wang, Y. Y. & Wu, M. W. Schottkybarrierinduced spin relaxation in spin injection. Phys. Rev. B 72, 153301 (2005).
Kubota, T. et al. Halfmetallicity and Gilbert damping constant in Co_{2}FexMn1−xSi Heusler alloys depending on the film composition. Appl. Phys. Lett. 94, 122504 (2009).
Kasai, S. et al. Magnetotransport and microstructure of Co_{2}Fe (Ga_{0.5}Ge_{0.5})/Cu lateral spin valves prepared by topdown microfabrication process. J. Appl. Phys. 115, 173912 (2014).
Winterlik, J. et al. Design Scheme of New Tetragonal Heusler Compounds for SpinTransfer Torque Applications and its Experimental Realization. Adv. Mater. 24, 6283 (2012).
Ouardi, S., Fecher, G. H., Felser, C. & Kübler, J. Realization of Spin Gapless Semiconductors: The Heusler Compound Mn_{2}CoAl. Phys. Rev. Lett. 110, 100401 (2013).
Chen, J. H. et al. Electronic structure, magnetism and phase stability of isostructural Ga_{2}MnCoGa_{2}MnV Heusler alloys from first principles. Computational Materials Science 89, 130 (2014).
Liu, E. K. et al. Stable magnetostructural coupling with tunable magnetoresponsive effects in hexagonal ferromagnets. Nat. Commun. 3, 873 (2012).
de Groot, R. A., Mueller, F. M., van Engen, P. G. & Buschow, K. H. J. New Class of Materials: HalfMetallic Ferromagnets. Phys. Rev. Lett. 50, 1983 (2014).
Luo, H. Z. et al. Electronic structure and magnetic properties of Fe_{2}YSi (Y=Cr, Mn, Fe, Co, Ni) Heusler alloys: a theoretical and experimental study. J. Phys. D: Appl. Phys. 40, 7121 (2007).
Suzukia, R. O. & Kyono, T. Thermoelectric properties of Fe_{2}TiAl Heusler alloys. J Alloys & Compds. 377, 38 (2004).
Bhat, I. H., Bhat, T. M. & Gupta, D. C. Magnetoelectronic and thermoelectric properties of some Febased Heusler alloys. J Phys. Chem. Solids 119, 251 (2018).
Wen, Y. H. et al. Large recovery strain in FeMnSibased shape memory steels obtained by engineering annealing twin boundaries. Nat. Commun. 5, 4964 (2014).
Khandy, S. A. & Gupta, D. C. First Principles understanding of Structural Electronic and Magnetic properties of new Quaternary Heusler alloy: FeVRuSi. Mater. Res. Express. 5, 056516 (2018).
Bilc, I. D., Hautier, G., Waroquiers, D., Rignanese, G. M. & Ghosez, P. LowDimensional Transport and Large Thermoelectric Power Factors in Bulk Semiconductors by Band Engineering of Highly Directional Electronic States. Phys. Rev. Lett. 114, 136601 (2015).
Tanaka, K. & Koiwa, M. SingleCrystal Elastic Constants of Intermetallic Compounds. Intermetallics 4, S29 (1996).
Murtaza, G. et al. Structural, Electronic, Optical and Thermodynamic Properties of Cubic REGa_{3} (RE=Sc or Lu) Compounds: Ab Initio Study. J. Alloys Compd. 597, 36 (2014).
Mouhat, F. & Coudert, F. X. Necessary and Sufficient Elastic Stability Conditions in Various Crystal Systems. Phys. Rev. B 90, 224104 (2014).
Khandy, S. A. & Gupta, D. C. Investigation of Structural, Magnetoelectronic and Thermoelectric response of Ductile SnAlO_{3} from Highthroughput DFT Calculations. Int. J Quantum Chem. 00, e25351, https://doi.org/10.1002/qua.25351, (2017).
Mir, S. H. et al. Static and Dynamical Properties of heavy actinide Monopnictides of Lutetium. Sci. Rep. 6, 29309 (2016).
Khandy, S. A. & Gupta, D. C. Structural, Elastic and Magnetoelectronic Properties of Halfmetallic BaNpO_{3} Perovskite. Mat. Chem. Phys. 198, 380 (2017).
Chen, X. Q., Niu, H., Li, D. & Li, Y. Intrinsic Correlation between Hardness and Elasticity in Polycrystalline Materials and Bulk Metallic Glasses. Intermetallics 19(9), 1275 (2011).
Pugh, S. F., XCII. Relations between the elastic moduli and the plastic properties of polycrystalline pure metals, Philos. Mag. Ser. 7(45), 823 (1954).
Khandy, S. A. & Gupta, D. C. Investigation of the transport, structural and mechanical properties of halfmetallic REMnO_{3} (RE=Ce and Pr) ferromagnets. RSC Adv. 6, 97641 (2016).
Frantsevich, I. N., Voronov, F. F. & Bokuta, S. A. In, Frantsevich, I. N. (Ed.), Elastic Constants and Elastic Moduli of Metals and Insulators. Naukova Dumka, Kiev. 60, 180 (1983).
Fine, M. E., Brown, L. D. & Marcus, H. L. Elastic Constants versus Melting Temperature in Metals. Scr. Metall. 18, 951 (1984).
Faleev, S. V. et al. Unified explanation of chemical ordering, the SlaterPauling rule, and halfmetallicity in full Heusler compounds. Phys. Rev. B 95, 045140 (2017).
Cai, Y., Bai, Z., Yang, M. & Feng, Y. P. Effect of interfacial strain on spin injection and spin polarization of Co_{2}CrAl/NaNbO_{3}/Co_{2}CrAl magnetic tunneling junction. EPL 99, 37001 (2012).
Cai, Y., Lan, J., Zhang, G. & Zhang, Y. W. Lattice vibrational modes and phonon thermal conductivity of monolayer MoS_{2}. Phy. Rev. B 89, 035438 (2014).
Cai, Y. et al. Giant Phononic Anisotropy and Unusual Anharmonicity of Phosphorene: Interlayer Coupling and Strain Engineering. Adv. Funct. Mater. 25, 2230 (2015).
Khandy, S.A., Islam, I., Gupta, D.C., Laref, A., Predicting the electronicstructure, magnetism, and transport properties ofnew Cobased Heusler alloys. Int J Energy Res. 1–8, https://doi.org/10.1002/er.4182 (2018).
Zhang, L. & Gao, Y. C. Electronic structures, magnetic properties and halfmetallicity in the Heusler alloy Hf_{2}VAl. Chinese Journal of Physics. 55(4), 1466 (2017).
Blaha, P., Schwarz, K., Sorantin, P. & Trickey, S. B. Fullpotential, linearized augmented plane wave programs for crystalline systems. Comput. Phys. Commun. 59, 399 (1990).
Blaha, P., Schwarz, K., Madsen, G.K.H., Kvasnicka, D & Luitz, J. WIEN2k, An Augmented Plane Wave + Local Orbitals Program for Calculating Crystal Properties ed; K. Schwarz (Wien, Austria: Techn. Universitaet Wien), (2001).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 77, 3865 (1996).
Tran, F. & Blaha, P. Accurate Band Gaps of Semiconductors and Insulators with a Semilocal ExchangeCorrelation Potential. Phys. Rev. Lett. 102, 226401 (2009).
Şaşıoğlu, E., Galanakis, I., Friedrich, C. & Blügel, S. Ab initio calculation of the effective onsite Coulomb interaction parameters for halfmetallic magnets. Phys. Rev. B 88, 134402 (2013).
Dudarev, S. L., Botton, G. A., Savrasov, S. Y., Humphreys, C. J. & Sutton, A. P. Electronenergyloss spectra and the structural stability of nickel oxide: An LSDA + U study. Phys. Rev. B 57, 1505 (1998).
Jamal, M. A Package for calculating elastic tensors of cubic Phases by using secondorder derivative with WIEN2k Package, http://www.WIEN2k.at/reg_user/unsupported/cubicelast/ (2012).
Gao, J., Zhao, J. & Ding, F. Transition Metal Surface Passivation Induced Graphene Edge Reconstruction. J. Am. Chem. Soc. 138(14), 4763 (2012).
Liu, X., Gao, J., Zhang, G. & Zhang, Y. W. MoS_{2}graphene inplane contact for high interfacial thermal conduction. Nano Research 10(9), 2944 (2017).
Gonze, X., Allan, D. C. & Teter, M. P. Dielectric tensor, effective charges, and phonons in αquartz by variational densityfunctional perturbation theory. Phys. Rev. Lett. 68, 3603 (1992).
Giannozzi, P. et al. Quantum ESPRESSO: a modular and opensource software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
Acknowledgements
One of the authors, A. Laref, wants to acknowledge the “Research Center of Female Scientific and Medical Colleges”, Deanship of Scientific Research, King Saud University for the financial support.
Author information
Authors and Affiliations
Contributions
S.A. Khandy conceived the study, carried out the calculations and wrote the manuscript. I. Islam and A. Laref gave some comments to improve the current form of manuscript. A. Laref also supplied the phonon calculations. All the authors contributed to the analysis and discussion for the results. D.C. Gupta and R. Khenata helped in reviewing this article.
Corresponding author
Ethics declarations
Competing Interests
The authors declare no competing interests.
Additional information
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Khandy, S.A., Islam, I., Gupta, D.C. et al. Lattice dynamics, mechanical stability and electronic structure of Febased Heusler semiconductors. Sci Rep 9, 1475 (2019). https://doi.org/10.1038/s4159801837740y
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4159801837740y
This article is cited by

Electronic, elastic, and thermodynamic properties of Cd0.75TM0.25S (TM = Os or Ir) alloys with the TBmBJ approach and hybrid density functional (HSE06)
Indian Journal of Physics (2024)

Exploring the electronic structure, mechanical behaviour, thermal and hightemperature thermoelectric response of CoZrSi and CoZrGe Heusler alloys
Scientific Reports (2023)

Effect of alloying Li on lithiumion batteries applicability of twodimensional TiN and TiC as novel electrode materials: a first principle study
Scientific Reports (2023)

Stability of silicon–tin alloyed nanocrystals with high tin concentration synthesized by femtosecond laser plasma in liquid media
Scientific Reports (2023)

Exploring the structural, electronic, optical properties and stability of Na2SrX (Si and Ge) fullHeusler alloys: A first principle investigation
Emergent Materials (2023)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.